Gives the broad overview of mechanical behaviour of the material.
Mechanical Properties of Solid Polymers
The properties of polymers are required firstly to select a material which enables desired performance of the plastics component under conditions of its application. Furthermore they are also essential in design work to dimension a part from a stress analysis or to predict the performance of a part under different stress situations involved. Knowledge of polymer properties is, as already mentioned in the preface, a prerequisite for designing and optimizing polymer processing machinery. In addition to the physical properties there are certain properties known as performance or engineering properties which correlate with the performance of the polymer under varied type of loading and environmental influences such as impact, fatigue, high and low temperature behavior and chemical resistance. The following sections deal with the physical as well as important performance properties of polymers.
1.1 Ideal SolidsIdeal elastic solids deform according to Hookean law which states that the stress is directly proportional to strain. The behavior of a polymer subjected to shear or tension can be described by comparing its reaction to an external force with that of an elastic solid under load. To characterize ideal solids, it is necessary to define certain quantities as follows :
1.2 Tensile PropertiesThe axial force Fn in Fig. 1.1 causes an elongation A/ of the sample of diameter d0 and length I0 fixed at one end. Following equations apply for this case: Engineering strain: (1.2.1)
Hencky strain: (1.2.2) Tensile stress: (1.2.3) Reference area: (1.2.4) Poisson's ratio: (1.2.5)
Fig. 1.1: Deformation of a Hookean solid by a tensile stress 
1.2.1 Stress-Strain BehaviorAs shown in Fig. 1.2 most metals exhibit a linear stress-strain relationship (curve 1), where as polymers being viscoelastic show a non-linear behavior (curve 2). When the stress is directly proportional to strain the material is said to obey Hooke's law. The slope of the straight line portion of curve 1 is equal to the modulus of elasticity. The maximum stress point on the curve, up to which stress and strain remain proportional is called the proportional limit (point P in Fig. 1.2) [I].
Strain z Fig. 1.2: Typical stress-strain curves of metals and polymers Most materials return to their original size and shape, even if the external load exceeds the proportional limit. The elastic limit represented by the point E in Fig. 1.2 is the maximum load which may be applied without leaving any permanent deformation of the material. If the material is loaded beyond its elastic limit, it does not return to its original size and shape, and is said to have been permanently deformed. On continued loading a point is reached at which the material starts yielding. This point (point Y in Fig. 1.2) is known as the yield point, where an increase in strain occurs without an increase in stress. It should however be noted that some materials may not exhibit a yield point. The point B in Fig. 1.2 represents break of the material.
Strain E Fig. 1.3: Secant modulus  Owing to their non-linear nature it is difficult to locate the straight line portion of the stress-strain curve for polymeric materials (Fig. 1.3). The secant modulus represents the
ratio of stress to strain at any point (S in Fig. 1.3) on the stress-strain diagram and is equal to the slope of the line OS. It is an approximation to a linear response over a narrow, but pre-specified and standard level of strain , which is usually 0.2%. The initial modulus is a straight line drawn tangent to the initial region of the stressstrain curve to obtain a fictive modulus as shown in Fig. 1.4. As this is ambiguous, the resin manufacturers provide a modulus with the stress, for example, G05 corresponding to a strain 0.5 % to characterize the material behavior on a practical basis (Fig. 1.4) , This stress G0 is also known as the proof stress. Nm m2 /
Sr i S tan
Fig. 1.4: Stress at a strain of 0.5% 
Fig. 1.5: Tensile stress diagram of a number of materials at 23C [ 4 ]: a: steel, b: copper, c: polycarbonate, d: PMMA, e: PE-HD, f: rubber, g: PE-LD, h: PVC-P
Stress-strain diagrams are given in Fig. 1.5 for a number of materials . It can be seen from Fig. 1.5 that the advantage of metals lies in their high strength, where as that of plastics lies in their high elongation at break. 1.2.2 Tensile Modulus According to Eq. (1.2.1) and Eq. (1.2.3) one obtains for the modulus of elasticity E which is known as Young's Modulus E = az/ 8 (1.2.6) The modulus of elasticity in a tension test is given in Table 1.1 for different polymers . Table 1.1: Guide Values of Modulus of Elasticity of Some Plastics  Material PE-LD PE-HD PP PVC-U PS ABS PC POM PA6 PA66 PMMA PET PBT PSU CA CAB Phenol-Formaldehyde-Resins Urea-Formaldehyde-Resins Melamin-Formaldehyde-Resins Unsaturated Polyester Resins Modulus of elasticity N mm'2 200/500 700/1400 1100/1300 1000/3500 3200/3500 1900/2700 2100/2500 2800/3500 1200/1400 1500/2000 2700/3200 2600/3100 1600/2000 2600/2750 1800/2200 1300/1600 5600/12000 7000/10500 4900/9100 14000/20000
The 3.5 % flexural stresses of thermoplastics obtained on a 3-point bending fixture (Fig. 1.6)  lie in the range 100 to 150 N mm"2 and those of thermosets from around 60 to 150 N mm"2 .
A pi d l a p le o d
Fig. 1.6: Three point bending fixture 
1.2.3 Effect of Temperature on Tensile StrengthThe tensile strength is obtained by dividing the maximum load (point M in Fig. 1.2) the specimen under test will withstand by the original area of cross-section of the specimen. Fig. 1.7 shows the temperature dependence of the tensile strength of a number of plastics .
1.3 Shear PropertiesFigure 1.8 shows the influence of a shear force Ft acting on the area A of a rectangular sample and causing the displacement AU. The valid expressions are defined by: Shear strain: (1.3.1) Shear stress (1.3.2)
1.3.1 Shear ModulusThe ratio of shear stress to shear strain represents the shear modulus G. From the equations above results: (1.3.3)
N mm2 psi Tensile stress Temperature0
Fig. 1.7: Temperature dependence of the tensile stress of some thermoplastics under uniaxial loading ; a: PMMA, b: SAN, c: PS, d: SB, e: PVC-U f: ABS, g: CA, h: PE-HD, i: PE-LD, k: PE-LD-V
Fig. 1.8: Deformation of a Hookean solid by shearing stress 
1.3.2 Effect of Temperature on Shear ModulusThe viscoelastic properties of polymers over a wide range of temperatures can be better characterized by the complex shear modulus G* which is measured in a torsion pendulum test by subjecting the specimen to an oscillatory deformation Fig. 1.9 . The complex shear modulus G* is given by the expression  (1.3.4) The storage modulus G' in Eq. (1.3.4) represents the elastic behavior associated with energy storage and is a function of shear amplitude, strain amplitude and the phase angle
5 between stress and strain. The loss modulus G" which is a component of the complex modulus depicts the viscous behavior of the material and arises due to viscous dissipation.
8 TM (t) IE Fig. 1.9: Torsion pendulum; Loading mode and sinusoidal angular displacement t  The tangent of the phase angle 8 is often used to characterize viscoelastic behavior and is known as loss factor. The loss factor d can be obtained from (1.3.5) The modulus-temperature relationship is represented schematically in Fig. 1.10 , from which the influence of the transition regions described by the glass transition temperature Tg and melting point Tm is evident. This kind of data provides information on the molecular structure of the polymer. The storage modulus G' which is a component of the complex shear modulus G* and the loss factor d are plotted as functions of temperature for high density polyethylene in Fig. 1.11 . These data for various polymers are given in the book .
HR AD B I TE RT L SL OI D
TUH OG SL OI D
VC U SOS I ML ET
R BE Y UBR
TEMPERATURE Fig. 1.10: Generalized relationship between deformation resistance and temperature for amorphous (solid line) and semi-crystalline (broken line) high polymers 
Dynamic shear modulus G'
Fig. 1.11: Temperature dependence of the dynamic shear modulus, G' and the loss factor d, obtained in the torsion pendulum test DIN 53445 : PE-HD (highly crystalline), PE-HD (crystalline), PE-LD (less crystalline)
1.4 Compressive PropertiesThe isotropic compression due to the pressure acting on all sides of the parallelepiped shown in Fig. 1.12 is given by the engineering compression ratio K . (1.4.1) where AV is the reduction of volume due to deformation of the body with the original volume F0.P P
Fig. 1.12: Hookean solid under compression 
Mechanical loss factor d
Table 1.2: Poisson ratio ju, density p, bulk modulus K and specific bulk modulus for some materials  Material Poisson ratio ju Density p at 200C g/cm3 7.8. 2.7 8.9 2.65 2.5 1.05 1.17 1.08 0.91 0.92 1 0.9 Bulk modulus K N/m2 1.66-1011 7-1010 1.344011 3.9-1010 3.7-1010 3-109 4.1-109 3.3-109 0.033-109 0.7-109 2-109 1.33-109 Specific bulk modulus KJp m2/s2 2.1-107 2.6107 1.5-107 1.47-107 1.494 O7 2.85407 3.5407 2.3407 0.044 O7 3.7407 24 O6 1.5406
Mild steel Aluminum Copper Quartz Glass Polystyrene Polymethylmethacrylate Polyamide 66 Rubber PE-LD Water Organic liquids
0.27 0.33 0.25 0.07 0.23 0.33 0.33 0.33 0.49 0.45 0.5 0.5
1.4.1 Bulk ModulusT